Share this document with a friend

Embed Size (px)

of 71
/71

Transcript

Rheology SGR Predictions Virtual Banding Outlook

Exploring soft glassy rheology:Mesoscopic analysis of simulation data and

effective temperature dynamics

Peter SollichA Barra, M E Cates, S M Fielding, P Hebraud, F Lequeux

King’s College London

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Soft glasses

Emulsions, dense colloidal suspensions, foams, microgels

Structural similarities: made up of squishy “particles”

Oil droplets [ignore coalescence], colloidal particles,air bubbles [ignore coarsening]

Typical particle scale µm, larger for foams, smaller for colloids

Particles have different shapes and sizes (polydisperse)

Particle packing is amorphous (disordered)

Metastable: kBT too small to make system ergodic & reachoptimal packing (crystalline, if polydispersity not too strong)

So glassy (repulsive glass) – but soft, can easily be made to flow

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Outline

1 Rheology: A reminder

2 Soft glasses: Phenomenology and SGR model

3 SGR predictions and model limitations

4 Comparison with simulations: Virtual strain analysis

5 Effective temperature dynamics, shear banding

6 Outlook

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Outline

1 Rheology: A reminder

2 Soft glasses: Phenomenology and SGR model

3 SGR predictions and model limitations

4 Comparison with simulations: Virtual strain analysis

5 Effective temperature dynamics, shear banding

6 Outlook

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Shear stress and strain

d

h

AF

Shear strain: γ = d/h, shear stress σ = F/A (really tensors)

Elastic solid: σ = Gγ, elastic (shear) modulus G

Newtonian fluid: σ = ηγ, viscosity η

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Linear rheology & viscoelasticity

Small strain increment (step) ∆γ at t = 0causes stress σ(t) = G(t)∆γ

G(t) = stress relaxation functionConstant for solid, spike ηδ(t) for fluid

Most materials are in between: viscoelastic

For short t, G(t) nearly constant (solid),but eventually → 0 (fluid)

Linear superposition of many small strain steps ∆γ = γ∆t:

σ(t) =∫ t

0G(t− t′)γ(t′) dt′

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Maxwell model

G

t

τ

Elastic solid and viscous fluid “in series” (spring & damper)

Common stress σ, elastic strain obeys σ = G0γel,viscous strain σ = ηγvisc

Total strain rate γ = γel + γvisc = σ/G0 + σ/η

Solve for small strain step (γ(t) = ∆γ δ(t)):

G(t) = G0 exp(−t/τ), τ = η/G0

Note η =∫∞0 G(t) dt, generally true if(!) flow with constant

strain rate is a linear perturbation

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Another Maxwell model

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Complex modulus

Experimentally, oscillatory measurements often easier

If γ(t) = γ0 cos(ωt) = γ0 Re eiωt, then

σ(t) = Re∫ t

0G(t− t′)iωγ0e

iωt′dt′ = Re G∗(ω)γ(t)

G∗(ω) = iω

∫ ∞

0G(t′′)e−iωt′′dt′′ for large t

Write complex modulus G∗(ω) = G′(ω) + iG′′(ω), then

σ(t) = G′(ω)γ0 cos(ωt)−G′′(ω)γ0 sin(ωt)

Elastic modulus G′(ω): in-phase part of stress

Viscous or loss modulus G′′(ω): out-of-phase (ahead by π/2)

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Complex modulus of Maxwell model

G’

ln G

ln ω1/τ

11

2G’’

G∗(ω) = iω×Fourier transform of G0 exp(−t/τ) = G0iωτ

1+iωτ

G′(ω) = G0ω2τ2

1 + ω2τ2, G′′(ω) = G0

ωτ

1 + ω2τ2

Single relaxation time gives peak in G′′(ω) at ω = 1/τ

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Nonlinear rheology

For most complex fluids, steady flow (rate γ) isnot a small perturbation, don’t get σ = ηγ

Flow curve σ(γ): stress in steady state

Often shear-thinning: downward curvature

Many other nonlinear perturbations:

large step stress or strainlarge amplitude oscillatory stress or strainstartup/cessation of steady shear etc

Most general description: constitutive equation

σ(t) = some function(al) of strain history [γ(t′), t′ = 0 . . . t]

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Outline

1 Rheology: A reminder

2 Soft glasses: Phenomenology and SGR model

3 SGR predictions and model limitations

4 Comparison with simulations: Virtual strain analysis

5 Effective temperature dynamics, shear banding

6 Outlook

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Soft glasses: Linear rheology

Complex modulus for dense emulsions (Mason Bibette Weitz 1995)

Almost flat G′′(ω): broad relaxation time spectrum, glassy

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Colloidal hard sphere glassesMason Weitz 1995

G′′(ω) again becomes flat as volume fraction increases

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Onion phasePanizza et al 1996

Vesicles formed out of lamellar surfactant phase

Again nearly flat moduli

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Microgel particlesPurnomo van den Ende Vanapalli Mugele 2008

G′′(ω) flat but with upturn at low frequencies

Aging: Results depend on time elapsed since preparation,typical of glasses

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Nonlinear rheology: Flow curves

γ

σ

.σy

σ

γ.

Flow curves typically well fitted by σ(γ)− σy ∼ γp (0 < p < 1)

Herschel-Bulkley if yield stress σy 6= 0,unsheared state = “glass”

Otherwise power law flow curve,unsheared state = “fluid” (but η = σ/γ →∞ for γ → 0)

Shear thinning: σ/γ decreases with γ

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

A non-glassy model for foam rheologyPrincen 1968

Ideal 2d foam (identical hexagonal cells), T = 0Apply shear: initially perfectly reversible response,stress increasesEventually interfaces rearrange, bubbles “slide”: global yieldProcess repeats under steady shearWe get: yield stressWe don’t get: broad relaxation time spectrum (Buzza Lu Cates

1995), aging

l

E

l

E

l

E’

l

E Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

SGR modelPS Lequeux Hebraud Cates 1997, PS 1998

How do we incorporate structural disorder?

Divide sample conceptually into mesoscopic elements

Each has local shear strain l, which increments withmacroscopic shear γ

Assumes strain rate γ uniform throughout system, but allowsfor variation in local strain and stress (compare STZ)

When strain energy 12kl2 reaches yield energy E,

element can yield and so reset to l = 0k = local shear modulus

If all elements have same E and k, this would essentially giveback the Princen model

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

SGR modelPS Lequeux Hebraud Cates 1997, PS 1998

New ingredient 1: disorder ⇒ every element has its own E

Initial distribution of E across elements depends onpreparation

When an element yields, it rearranges into new localequilibrium structure ⇒ acquires new E from somedistribution ρ(E) ∝ e−E/E (assume no memory of previous E)

New ingredient 2: Yielding is activated by an effectivetemperature x, to model interactions between elements

x should be of order E, � kBT (negligible)

Model implicitly assumes low frequency/slow shear:yields are assumed instantaneous, no solvent dissipation

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Sketch

l

E

l

E

l

E’

l

E

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Dynamical equation for SGR

P (E, l, t): probability of an element having yield energy Eand local strain l at time t

Master equation (Γ0 = attempt rate for yields)

P (E, l, t) = −γ∂P

∂lconvection of l

− Γ0e−(E−kl2/2)/xP elements yield

+ Γ(t)ρ(E)δ(l) elements reborn after yield

where Γ(t) = Γ0〈e−(E−kl2/2)/x〉 = average yielding rate

Macroscopic stress σ(t) = k 〈l〉Given initial condition P (E, l, 0) and strain history (input)can in principle calculate stress (output)

We’ll rescale E, t, l so that E = Γ0 = k = 1;this means also typical yield strains are 1

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Equilibrium & glass transition in the trap model

Master equation for P (E, t) in absence of flow (l = 0)

P (E, t) = −e−E/xP + Γ(t)ρ(E)

P (E, t) approaches equilibrium Peq(E) ∝ exp(E/x)ρ(E)for long t (Boltzmann distribution; E is measured downwards)

Get glass transition if ρ(E) has exponential tail(possible justification from extreme value statistics)

Reason: for low enough x, Peq(E) cannot be normalized

For ρ(E) = e−E this transition happens at x = 1For x < 1, system is in glass phase; never equilibrates

Aging: evolution into ever deeper traps

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Outline

1 Rheology: A reminder

2 Soft glasses: Phenomenology and SGR model

3 SGR predictions and model limitations

4 Comparison with simulations: Virtual strain analysis

5 Effective temperature dynamics, shear banding

6 Outlook

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Linear response in the fluid phase

Calculation yields average of Maxwell models:

G∗(ω) =⟨

iωτ1+iωτ

⟩, average is over Peq(τ), τ = exp(E/x)

For large x, get usual power-law dependences for small ω

But near x = 1 get G′ ∼ G′′ ∼ ωx−1: both become flat

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Linear response: AgingSollich PS Cates 2000

Conceptual issue: with aging, G∗(ω) → G∗(ω, t, tw)G∗(ω, t, tw) could depend on final time tand start time tw of shear

Luckily, dependence on tw is weak: G∗(ω, t)Find simple aging 1/ω ∼ t: G∗(ω, t) ∼ 1− (iωt)x−1

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Linear response: Aging

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Comparison with experiments on microgel particlesPurnomo van den Ende Vanapalli Mugele 2008

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Flow curve

x=2

x=1

Calculation: steady state, so set P = 0 in master equation,integrate differential eqn for l; Γ from normalizationThree regimes for small γ:

σ ∼

γ for 2 < x : Newtonianγx−1 for 1 < x < 2 : power lawσy(x) + γ1−x for x < 1 : Herschel-Bulkley

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Yield stress

Yield stress increases continuously at glass transition

Compare MCT prediction: discontinuous onset of yield stress

Physics?Elastic networks/stress chains vs caging?Jamming transition vs glass transition?

Could e.g. emulsions exhibit both transitions?

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

General nonlinear rheologyExample: Large amplitude oscillatory strain

Close to but above glass transition (x = 1.1, ω = 0.01)

Increasing strain amplitude gives stronger nonlinearities

Hysteresis-like loops

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Large oscillatory strain: Complex modulus

G′′ first increases with amplitude, becomes larger than G′

Large strain fluidizes an initially predominantly elastic system

Compare experiments on colloidal hard spheres (right)

Quantitative comparison for foam(Rouyer Cohen-Addad Hohler PS Fielding 2008)

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

SGR predictions: Summary

Flow curves: Find both Herschel-Bulkley (x < 1) andpower-law (1 < x < 2)

Viscoelastic spectra G′, G′′ ∼ ωx−1 are flat near x = 1In glass phase (x < 1) find rheological aging,loss modulus G′′ ∼ (ωt)x−1 decreases with age t

Steady shear always interrupts aging,restores stationary state

Large amplitude G′ and G′′ show fluidization behavioursimilar to experiments

Stress overshoots in shear startup,linear and nonlinear creep,rejuvenation and overaging(Lequeux, Viasnoff, McKenna, Cloıtre, Roettler . . . )

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Limitations of SGR model

Scalar model with ideal local elasticity up to yield –both can be fixed (Cates PS 2004)

No spatial information: geometry of stress redistributionmight be important, also non-affine flow

Length scale of elements: needs to be large enough to allowlocal strain and stress to be defined, but otherwise unspecified

Interpretation of effective temperature x?Link to material parameters?Should have own dynamics? (see later)

What sets fundamental time scale (attempt rate for yielding)?

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Thermodynamic interpretation of SGR model

Can interpret SGR within Bouchbinder & Langernon-equilibrium thermodynamics framework

Slow degrees of freedom Λ used to characterizenon-equilibrium state: P (E, l) (finite but large nr. of bins)

Internal energy and entropy associated with these:

UΛ(Λ) = (V/ve)∫

dE dl P (E, l)(12kvel

2 − E)

SΛ(Λ) = −(V/ve)∫

dE dl P (E, l) (ln[P (E)/ρ(E)]− 1)

Note: no entropy for l-distribution as l-dynamics is “slaved”to E-dynamics (times of yields)

Thermodynamic consistency (2nd law) requires that x mustbe identical to thermodynamic temperature χ of slow d.o.f.

Most plausible choices of yield rates Γ(E, l) are allowed

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Comparison to Jim Langer’s “simple” SGR model

What would we get only with effective temperature dynamicsand a Maxwell model with temperature-dependent relaxationtime?

χ = . . . e−1/χ + . . . (T − χ), σ = kγ − . . . e−1/χσ

G′′(ω) in steady state always Maxwell, not broad

Broadening of spectra can arise only from aging effects

Also no nonlinearities in strain amplitude, so no solid-liquidcrossover in oscillatory strain

Interesting flow curves only from additional flow-dependentdriving terms for χ

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Outline

1 Rheology: A reminder

2 Soft glasses: Phenomenology and SGR model

3 SGR predictions and model limitations

4 Comparison with simulations: Virtual strain analysis

5 Effective temperature dynamics, shear banding

6 Outlook

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Simulations to the rescue?

Can we use simulation data to:

See how far the SGR model represents physical reality?

Get better understanding of model parameters?

Tell us where we should improve the model?

Need to develop method for explicit coarse-graining ofsimulation data

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Defining elements

Focus on d = 2 (d = 3 can be done but more complicated)

Make elements circular to minimize boundary effects

Position circle centres on square lattice to cover all of thesample (with some overlap)

Once defined, element is co-moving with strain:always contains same particles

Avoids sudden change of element properties when particlesleave/enter, but makes sense only up to moderate ∆γ

Measuring average stress in an element is easy but how do weassign strain l, yield energy etc for a given snapshot?

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Virtual strain analysis

Deliberately want local yield points etc: interaction betweenelements is accounted for separately within model

Cannot “cut” an element out of sample and then strain untilyield – unrealistic boundary condition

Idea: Use rest of sample as a frame

Deform the frame affinely to impose a virtual strain γ

Particles inside element relax non-affinely to minimize energy

Gives energy landscape ε(γ) of element

Yield points are determined (for γ > 0 and < 0) by checkingfor reversibility for each small ∆γ (adaptive steps)

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 1

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 2

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 3

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 4

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 5

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 6

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 7

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 8

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Example: Virtual strain sequence 9

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Element energy landscape

0.5

0.55

0.6

0.65

0.7

0.75

0.8

-0.06 -0.05 -0.04 -0.03 -0.02 -0.01 0 0.01 0.02 0.03

ε

γ˜

l

∆E+

γ+

E+

εmin

Extract: minimum energy εmin, strain away from local minimuml = −γmin, yield strains γ±, yield barriers E±

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Local modulus

Quadratic fit of energy near minimum, or linear fit of stress,gives local modulus k

-0.4

-0.3

-0.2

-0.1

0

0.1

0.2

0.3

0.4

-0.06 -0.05 -0.04 -0.03 -0.02 -0.01 0 0.01 0.02 0.03

σ

˜γ

l

k(˜γ+l)

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Systems studied

Polydisperse Lennard-Jones mixtures (Tanguy et al), quenchedto low temperatures (T = 0.005 � Tg)

Low shear rates γ ∼ 10−3; N = 104 particles at ρ = 0.95Steady shear driven from the walls (created by “freezing”particles in top/bottom 5% some time after quench)

Check for stationarity & affine shape of velocity profilebefore taking data

Each element contains ≈ 40 particles (diameter = 7):large enough to have near-parabolic energy landscape,small enough to avoid multiple local yield events inside oneelement

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Simulation demo

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Close-up

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Results: Yield energy distribution

0

20

40

60

80

100

120

140

160

0 20 40 60 80 100 120 140 160 180

P(E

)

bins

Exponential tail; detailed form can be fitted by SGR model

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Yield strain distributions

0

0.01

0.02

0.03

0.04

0.05

0.06

0.07

0.08

-0.15 -0.1 -0.05 0 0.05 0.1 0.15

P(γ

-,γ+

)

γ-,γ+

γ-γ+

Symmetric as assumed in SGR; gap around 0 or maybe power-lawapproach (exponent ≈ 4)

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Modulus distribution

0

0.01

0.02

0.03

0.04

0.05

0.06

0.07

0.08

0.09

150 200 250 300 350 400

P(K

)

K

Clear spread; not constant as assumed in model.But yield strains γ± still controlled by E±; no correlation with k

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Local strain distribution

0

0.02

0.04

0.06

0.08

0.1

0.12

0.14

-0.04 -0.02 0 0.02 0.04 0.06 0.08

P(l)

strain

Negative l, need to extend SGR to allow frustration: l 6= 0 afteryield (δ(l) → ρ(l|E) ∝ (1− kl2/2E)b – but thermodynamics then

broken?)

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Dynamics: Evolution of local strain with time

-0.005

0

0.005

0.01

0.015

0.02

0.025

0.03

0.035

0.04

0.045

0 0.01 0.02 0.03 0.04 0.05 0.06

l

γ

Typical sawtooth shape assumed by SGR

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Change in other landscape propertiesExample of modulus

250

260

270

280

290

300

310

320

330

340

0 0.01 0.02 0.03 0.04 0.05 0.06

K

γ-0.005

0

0.005

0.01

0.015

0.02

0.025

0.03

0.035

0.04

0.045

0 0.01 0.02 0.03 0.04 0.05 0.06

l

γ

Stays largely constant between yields as expected;same for yield barriers etc

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Comparing real and virtual deformationsPrimary yield

0.2

0.25

0.3

0.35

0.4

0.45

0.5

0.55

0.6

0.65

0.7

0 0.01 0.02 0.03 0.04 0.05

ε

γ˜

0

1

2

3

4

5

6

7

8

9

1011

BA

realvirtual

Curve: virtual energy landscape.Vertical lines: Real ε versus l − l0 for uniform steps ∆γGood match, even for energy drop after yield

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Comparing real and virtual deformations (cont)Induced yield

0.45

0.5

0.55

0.6

0.65

0.7

0.75

0.8

0.85

-0.01 0 0.01 0.02 0.03 0.04 0.05 0.06

ε

γ˜

0 1 23

4

5

6

7

8

9

10 11B

A

realvirtual

Curve: virtual energy landscape.Vertical lines: Real ε versus l − l0 for uniform steps ∆γ

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Summary for virtual strain analysis

Virtual strain method for assigning local strains, yield energies

Generic: can be used on configurations produced by any(low-T ) simulation

Steady state distributions in shear flow seem in line with SGR(detailed fits in progress), though e.g. local modulus 6= const

Dynamics of local strain has typical sawtooth shape; localstrain rate is of same order as global one but not identical

Energy landscapes for real and virtual deformations match(but not purely quadratic)

To do: analysis of induced yield events – well modelled byeffective temperature?

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Outline

1 Rheology: A reminder

2 Soft glasses: Phenomenology and SGR model

3 SGR predictions and model limitations

4 Comparison with simulations: Virtual strain analysis

5 Effective temperature dynamics, shear banding

6 Outlook

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Effective temperature dynamicsFielding Cates PS 2008

Shouldn’t effective temperature x be determinedself-consistently by dynamics?

To allow for potential shear banding, split samplein y (shear gradient)-direction

Separate SGR model for each y, with x(y)Relaxation-diffusion dynamics:

τxx(y) = −x(y) + x0 + S(y) + λ2 ∂2x

∂y2

x is “driven” by energy dissipation rate:S = a〈l2 exp(−[(E − l2/2)/x])〉Assume that x equilibrates (locally) quickly: τx → 0

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Flow curvea = 2, x0 = 0.3

Steady state: x = x0 + 2aσ(x, γ)γShear startup with imposed mean γ across sample:shear banding

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Nature of banded statea = 2, x0 = 0.3, γ = 0.05, 0.1, 0.2

“Hot” band: γ > 0, ergodic

“Cold” band: γ = 0, aging

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Viscosity bifurcation at imposed stressCoussot, Bonn, . . .

σtw

Plot instantaneous viscosity η = σ/γ

Sample only reaches steady flow when σ is large enough

Depends on age tw when stress is applied

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Variation of driving term for x

x now driven by yield rate, S ∝ 〈exp(−[(E − l2/2)/x])〉Hysteresis in shear rate sweep: banding on way up,stay on fluid branch on way down

Resembles data for multi-arm polymers (Holmes Callaghan

Vlassopoulos Roovers 2004)

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Outline

1 Rheology: A reminder

2 Soft glasses: Phenomenology and SGR model

3 SGR predictions and model limitations

4 Comparison with simulations: Virtual strain analysis

5 Effective temperature dynamics, shear banding

6 Outlook

Peter Sollich (King’s College London) Exploring soft glassy rheology

Rheology SGR Predictions Virtual Banding Outlook

Summary & Outlook

Trap models for aging dynamics in glasses, focus on activation

SGR model adds strain to this & re-interprets trap depths asyield energies

Reproduces much (not all) of rheological behaviour of softglasses

. . . and some cytoskeletal rheology(?)

Virtual strain method allows detailed comparison withsimulations: some encouraging agreement, but also suggestsmodifications

Dynamics of x: phenomenological models useful, but toomuch choice? Thermodynamic approach could fix driving term

To do: linking to other approaches (STZ, Picard et al);coarse-graining from “microscopic” models?

Peter Sollich (King’s College London) Exploring soft glassy rheology

Recommended